Ultrafast nano-oscillators based on interlayer-bridged carbon nanoscrolls
© Zhang and Li; licensee Springer. 2011
Received: 29 May 2011
Accepted: 25 July 2011
Published: 25 July 2011
We demonstrate a viable approach to fabricating ultrafast axial nano-oscillators based on carbon nanoscrolls (CNSs) using molecular dynamics simulations. Initiated by a single-walled carbon nanotube (CNT), a monolayer graphene can continuously scroll into a CNS with the CNT housed inside. The CNT inside the CNS can oscillate along axial direction at a natural frequency of tens of gigahertz. We demonstrate an effective strategy to reduce the dissipation of the CNS-based nano-oscillator by covalently bridging the carbon layers in the CNS. We further demonstrate that such a CNS-based nano-oscillator can be excited and driven by an external AC electric field, and oscillate at more than 100 GHz. The CNS-based nano-oscillators not only offer a feasible pathway toward ultrafast nano-devices but also hold promise to enable nanoscale energy transduction, harnessing, and storage (e.g., from electric to mechanical).
Keywordscarbon nanoscroll graphene carbon nanotube nano-oscillator molecular dynamics
Significant research progress on graphene in past several years has enabled the exploration of carbon nanoscrolls (CNSs) [1–3], a one-dimensional carbon nanomaterial that is distinct from carbon nanotubes (CNTs). A CNS is formed by rolling up a monolayer graphene into a spiral multilayer nanostructure, whose core size is highly tunable by relative sliding between adjacent layers [4, 5]. In other words, a CNS is topologically open, fundamentally distinct from a tubular CNT, which is topologically closed (e.g., whose core size can only be changed slightly by stretching the carbon-carbon (C-C) bonds). The open and highly tunable structure of CNSs, combining with the exceptional mechanical and electronic properties inherited from the basal graphene [6–9], has inspired an array of novel nano-device applications, such as hydrogen storage medium [10, 11], water and ion channels , radially breathing nano-oscillators , and translational nano-actuators . In this paper, we demonstrate ultrafast CNS-based axial nano-oscillators that operate at frequencies from tens of gigahertz to more than 100 GHz, using molecular dynamic (MD) simulations.
It has been recently demonstrated that a CNT of suitable diameter can initiate the scrolling of a monolayer graphene on a substrate into a CNS . The CNT near the edge of the graphene can help overcome the initial energy barrier for the scrolling of graphene. Once the scrolling is initiated, the graphene can spontaneously roll up into a CNS. The resulting CNS/CNT nanostructure has the two ends of the CNS naturally open and a CNT housed inside the CNS (e.g., Figure 1b). Similar scrolling of a graphene oxide layer initiated by a MWCNT has been experimentally demonstrated recently . As to be detailed later, when the CNT is displaced partially out of the CNS along the axial direction, the van der Waals force acting on the two ends of the CNT is not balanced and the resultant force on the CNT serves as the restoring force to pull the CNT back into the CNS. Given the ultralow CNT-CNS friction similar to the inter-tube friction in a MWCNT, the CNT in the CNS is shown to be able to oscillate at a frequency of tens of gigahertz. In this paper, we use molecular dynamics simulations to perform systematic investigation of the characteristics of the ultrafast oscillation of the abovementioned CNS-based axial nano-oscillators. We propose a feasible strategy to significantly reduce the energy dissipation of the CNS-based nano-oscillators. We further demonstrate that the CNS-based nano-oscillators can be excited by an external AC electrical field and oscillate at a frequency more than 100 GHz. A distinct advantage of the CNS-based nano-oscillators against the MWCNT-based ones is as follows. The CNT and the basal graphene are fabricated separately before the scrolling process. For example, the CNT and the graphene can be treated differently and thus possess different features, such as defects, chirality, and polarization. These features make it possible to significantly enhance the performance of the CNS-based axial nano-oscillators, as to be detailed later in this paper. With the ever maturing fabrication technique of high-quality graphene, CNS-based axial nano-oscillators hold promise to become a viable approach to achieving nanoscale gigahertz mechanical oscillators. In particular, the excitation of CNS-based nano-oscillators under external interferences demonstrates their great potential as nanoelectromechanical systems (NEMS) for nanoscale energy transduction (e.g., from electrical and/or magnetic to mechanical), harvesting, and storage (e.g., as mechanical oscillation).
Results and discussions
CNT-initiated scrolling of graphene into a CNS
Initiated by the CNT, the graphene first separates from the substrate and curls up to wrap the CNT (Figure 2b). Once the overlap between the left edge and the flat portion of the graphene forms (Figure 2c), graphene starts to scroll continuously into a CNS (Figure 2d) with the CNT housed inside. An additional movie file shows the CNT-initiated scrolling of graphene into a CNS (see Additional file 1). Figure 2e shows the decrease of the total potential energy due to the graphene wrapping the CNT and further scrolling into a CNS. Our simulations show that there is no appreciable difference between the scrolling of a pristine graphene (without any defects) and that of a graphene with defects. For example, the graphene shown in Figure 2 has patterned vacancies along three parallel lines, the effect of which is to be detailed later.
Oscillation of a CNT housed inside a naturally formed CNS
To further decipher the coupled oscillation of the CNS/CNT nanostructure, we define two oscillation amplitudes: the absolute amplitude which is the axial distance from the left end of the CNT to the outermost atom at the left end of the CNS (which is fixed) and the relative amplitude which is the axial distance from the left end of the CNT to the innermost atom at the left end of the CNS (which moves as the CNS oscillates). Figure 3b, d plot the absolute and relative amplitudes as the function of simulation time, respectively. While the absolute amplitude captures the oscillation of the CNT, the relative amplitude characterizes the coupled oscillation of the CNS/CNT nanostructure, which is more irregular and decays faster. Fast Fourier Transform (FFT) analysis is also performed for the first 500 ps of the oscillation. FFT of the absolute amplitude shows a peak at 29.4 GHz (Figure 3c), which represents the frequency of CNT oscillation. By contrast, FFT of the relative amplitude shows two peaks, 29.4 and 50.9 GHz, respectively (Figure 3e). While the first peak corresponds to the frequency of CNT oscillation inside the CNS, the second peak reveals the frequency of the CNS self-oscillation. The higher frequency of the CNS self-oscillation results from the restoring force contributed by both the non-bonded van der Waals force among carbon layers and the covalent C-C bonding force in the basal graphene.
Oscillation of a CNT housed inside an interlayer-bridged CNS
While the ultrafast oscillation of the CNT inside the CNS at tens of gigahertz is encouraging, the quick dissipation and rather irregular behavior of the oscillation definitely limit the potential application of CNS-based nano-oscillators as NEMS devices. The quick dissipation and irregular oscillation result from the coupled oscillation, during which the kinetic energy of the CNT is continuously transduced into the self-oscillation of the CNS and then dissipates by the friction due to interlayer sliding. To address this issue, we next demonstrate a feasible and effective strategy to suppress the relative interlayer sliding in the CNS, which can lead to a much more sustainable ultrafast CNS-based nano-oscillator.
Both simulations and experiments have shown that when a MWCNT is treated by ion irradiation, some carbon atoms can be knocked off, leaving vacancies in the tubes of the MWCNT . Upon heating, the carbon atoms near the vacancies tend to form covalent bonds with other similar carbon atoms in a neighboring tube, driven by the reduction of high-energy dangling bonds of these carbon atoms. As a result, the tubes in the MWCNT are covalently bridged, leading to a significant increase of the inter-tube shear rigidity of the MWCNT. In other words, the relative inter-tube sliding in such a bridged MWCNT involves breaking the covalent C-C bridging bonds, thus is energetically unfavorable. The ion irradiation induced vacancies are also used to facilitate the bridging bond formation among SWCNTs to form CNT bundles [28, 29]. Inspired by these previous studies, next we demonstrate that vacancies can facilitate the formation of interlayer bridging bonds in a CNS, which in turn can effectively suppress the interlayer relative sliding in the CNS.
Effects of temperature and commensuration on the nano-oscillator performance
Oscillation of the CNS/CNT nano-oscillator excited and driven by an external electric field
To conclude, we demonstrate a new type of ultrafast axial nano-oscillators based on CNS. Such a nano-oscillator consists of a SWCNT that is housed inside a CNS, which can be feasibly formed by the SWCNT-initiated scrolling of a basal monolayer graphene. The unique topological structure of the CNS-based nano-oscillator offers a viable pathway to fabricating ultrafast axial nano-oscillators, addressing a significant challenge that still remains for the previously proposed MWCNT-based axial nano-oscillator. We propose an effective and feasible strategy to reduce the oscillation dissipation of the CNS-based nano-oscillators by introducing interlayer bridging bonds in the CNS. The performance of the resulting bridged-CNS-based nano-oscillators is comparable or modestly better than the MWCNT-based ones. We further demonstrate the highly sustainable oscillation of the bridged-CNS-based nano-oscillators that can be excited and driven by an external AC electric field. With the ever maturing fabrication of high-quality monolayer graphene and nanofabrication technique of patterning nanoscale building blocks, we envision a novel approach to harnessing and storing energy at nanoscale and over large area, enabled by distributing CNS-based nano-oscillators on an electronic surface.
carbon nanoscroll: SWCNT: single-walled carbon nanotube
double-walled carbon nanotube
multi-walled carbon nanotube
This work is supported by the National Science Foundation (grant no. 1069076), University of Maryland General Research Board Summer Research Award, and Maryland NanoCenter at the University of Maryland, College Park. ZZ also thanks the support of A. J. Clark Fellowship and UMD Clark School Future Faculty Program.
- Viculis LM, Mack JJ, Kaner RB: A chemical route to carbon nanoscrolls. Science 2003, 299: 1361. 10.1126/science.1078842View Article
- Shioyama H, Akita T: A new route to carbon nanotubes. Carbon 2003, 41: 179–181. 10.1016/S0008-6223(02)00278-6View Article
- Xie X, Ju L, Feng X, Sun Y, Zhou R, Liu K, Fan S, Li Q, Jiang K: Controlled fabrication of high-quality carbon nanoscrolls from monolayer graphene. Nano Lett 2009, 9: 2565–2570. 10.1021/nl900677yView Article
- Braga SF, Coluci VR, Legoas SB, Giro R, Galvao DS, Baughman RH: Structure and dynamics of carbon nanoscrolls. Nano Lett 2004, 4: 881–884. 10.1021/nl0497272View Article
- Shi XH, Pugno NM, Gao HJ: Tunable core size of carbon canoscrolls. J Comput Theor Nanosci 2010, 7: 517–521. 10.1166/jctn.2010.1387View Article
- Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric field effect in atomically thin carbon films. Science 2004, 306: 666–669. 10.1126/science.1102896View Article
- Zhang YB, Tan YW, Stormer HL, Kim P: Experimental observation of the quantum Hall effect and Berry's phase in graphene. Nature 2005, 438: 201–204. 10.1038/nature04235View Article
- Lee C, Wei X, Kysar JW, Hone J: Measurement of the elastic properties and intrinsic strength of monolayer graphene. Science 2008, 321: 385–388. 10.1126/science.1157996View Article
- Neto AHC, Guinea F, Peres NMR, Novoselov KS, Geim AK: The electronic properties of graphene. Rev Mod Phys 2009, 81: 109–154. 10.1103/RevModPhys.81.109View Article
- Mpourmpakis G, Tylianakis E, Froudakis GE: Carbon nanoscrolls: a promising material for hydrogen storage. Nano Lett 2007, 7: 1893–1897. 10.1021/nl070530uView Article
- Coluci VR, Braga SF, Baughman RH, Galvao DS: Prediction of the hydrogen storage capacity of carbon nanoscrolls. Phys Rev B 2007, 75: 6.
- Shi XH, Cheng Y, Pugno NM, Gao HJ: Tunable water channels with carbon nanoscrolls. Small 2010, 6: 739–744. 10.1002/smll.200902286View Article
- Shi XH, Pugno NM, Cheng Y, Gao HJ: Gigahertz breathing oscillators based on carbon nanoscrolls. Appl Phys Lett 2009, 95: 163113–163113. 10.1063/1.3253423View Article
- Shi XH, Cheng Y, Pugno NM, Gao HJ: A translational nanoactuator based on carbon nanoscrolls on substrates. Appl Phys Lett 2010, 96: 517–521.
- Zheng QS, Jiang Q: Multiwalled carbon nanotubes as gigahertz oscillators. Phys Rev Lett 2002, 88: 045503.View Article
- Legoas SB, Coluci VR, Braga SF, Coura PZ, Dantas SO, Galvao DS: Molecular-dynamics simulations of carbon nanotubes as gigahertz oscillators. Phys Rev Lett 2003, 90: 055504.View Article
- Rivera JL, McCabe C, Cummings PT: Oscillatory behavior of double-walled nanotubes under extension: a simple nanoscale damped spring. Nano Lett 2003, 3: 1001–1005. 10.1021/nl034171oView Article
- Ershova OV, Lozovik YE, Popov AM, Bubel ON, Poklonskii NA, Kislyakov EF: Control of the motion of nanoelectromechanical systems based on carbon nanotubes. Phys Solid State 2007, 49: 2010–2014. 10.1134/S1063783407100332View Article
- Coluci VR, Timoteo VS, Galvao DS: Thermophoretically driven carbon nanotube oscillators. Appl Phys Lett 2009, 95: 253103. 10.1063/1.3276546View Article
- Kang JW, Song KO, Hwang HJ, Jiang Q: Nanotube oscillator based on a short single-walled carbon nanotube bundle. Nanotechnology 2006, 17: 2250–2258. 10.1088/0957-4484/17/9/030View Article
- Zhang Z, Li T: Carbon nanotube initiated formation of carbon nanoscrolls. Appl Phys Lett 2010, 97: 081909. 10.1063/1.3479050View Article
- Kim YK, Min DH: Preparation of scrolled graphene oxides with multi-walled carbon nanotube templates. Carbon 2010, 48: 4283–4288. 10.1016/j.carbon.2010.07.039View Article
- Brenner DW, Shenderova OA, Harrison JA, Stuart SJ, Ni B, Sinnott SB: A second-generation reactive empirical bond order (REBO) potential energy expression for hydrocarbons. J Phys: Condens Matter 2002, 14: 783–802. 10.1088/0953-8984/14/4/312
- Stuart SJ, Tutein AB: Harrison, J. A. A reactive potential for hydrocarbons with intermolecular interactions. J Chem Phys 2000, 112: 6472–6486. 10.1063/1.481208View Article
- Plimpton S: Fast parallel algorithms for short-range molecular dynamics. J Comput Phys 1995, 117: 1–19. 10.1006/jcph.1995.1039View Article
- Coluci VR, Legoas SB, de Aguiar MAM, Galvao DS: Chaotic signature in the motion of coupled carbon nanotube oscillators. Nanotechnology 2005, 16: 583–589. 10.1088/0957-4484/16/4/041View Article
- Krasheninnikov AV, Banhart F: Engineering of nanostructured carbon materials with electron or ion beams. Nat Mater 2007, 6: 723–733. 10.1038/nmat1996View Article
- Kis A, Csanyi G, Salvetat JP, Lee TN, Couteau E, Kulik AJ, Benoit W, Brugger J, Forro L: Reinforcement of single-walled carbon nanotube bundles by intertube bridging. Nat Mater 2004, 3: 153–157. 10.1038/nmat1076View Article
- da Silva AJR, Fazzio A, Antonelli A: Bundling up carbon nanotubes through Wigner defects. Nano Lett 2005, 5: 1045–1049. 10.1021/nl050457cView Article
- Guo WL, Guo YF, Gao HJ, Zheng QS, Zhong WY: Energy dissipation in gigahertz oscillators from multiwalled carbon nanotubes. Phys Rev Lett 2003, 91: 125501.View Article
- Xu ZP: Energy dissipation in the double-walled carbon nanotube based mechanical oscillators. J Comput Theor Nanosci 2008, 5: 655–658.
- Zhao Y, Ma CC, Chen GH, Jiang Q: Energy dissipation mechanisms in carbon nanotube oscillators. Phys Rev Lett 2003, 91: 175504.View Article
- Zhao XG, Cummings PT: Molecular dynamics study of carbon nanotube oscillators revisited. J Chem Phys 2006, 124: 134705. 10.1063/1.2185623View Article
- Kang JW, Song KO, Kwon OK, Hwang HJ: Carbon nanotube oscillator operated by thermal expansion of encapsulated gases. Nanotechnology 2005, 16: 2670–2676. 10.1088/0957-4484/16/11/034View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.